# Estimation of C* Integral for Mismatched Welded Compact Tension Specimen

^{*}

## Abstract

**:**

## 1. Introduction

_{2}emissions in the chemical and petrochemical industries and in thermal power plants. Increasing the operating temperatures of the plant increases the energy efficiency, thus reducing CO

_{2}emissions. Higher operating temperatures and higher stresses increase the risk of welded structure failure due to creep conditions. It is therefore necessary to develop a method to predict the CCG in welded joints [3].

## 2. Numerical Analysis

#### 2.1. Geometry and Loading

^{−3/2}.

#### 2.2. Material Properties

_{BM}= 1 × 10

^{−20}(MPa)

^{−n}h

^{−1}and n

_{BM}= 7. To investigate the influence of material constraints on the C* integral in welded joints, different configurations of material mismatch in creep strain rate of BM, WM and HAZ were designed. The material creep properties for HAZ and WM were chosen so that the creep strain rate was lower or higher than that of BM. This was achieved by varying the constant A. The creep exponent n for BM, WM and HAZ was identical (n

_{BM}= n

_{WM}= n

_{HAZ}= 7). The effect of the mismatch in the creep properties for WM and HAZ relative to BM is expressed by the mismatch factor. These mismatch factors are defined as follows [18]:

_{WM}and MF

_{HAZ}factors are 10, 1 and 0.1, respectively. Thus, in order to investigate the effect of material constraints on the C* integral, nine possible combinations of material mismatch were considered, as shown in Table 1.

#### 2.3. Finite Element Analysis

_{I}and C* obtained by FE analyses with analytical solutions for CT specimen [22,23]. It is evident that the FE results provide confidence in the FE analyses for elastic and steady-state creep conditions.

## 3. Results and Discussion

_{HAZ}, MF

_{WM}and W/h on the factor φ for the ratio a/W = 0.5. It can be seen that MF

_{HAZ}has a strong influence on the factor φ for the considered values of MF

_{WM}and W/h. Values of φ are highest for creep-soft HAZ (MF

_{HAZ}= 0.1). It can be seen that these values are significantly higher than one, meaning that the C* integral is lower than the C* integral for a homogeneous CT specimen. A larger C* integral causes a higher rate of CCG. For a given value of MF

_{HAZ}, the factor φ is higher if MF

_{WM}is lower. For creep-hard HAZ (MF

_{HAZ}= 10), the values of φ are mostly lower than one, meaning that the C* integral is less than the C* integral for a homogeneous CT specimen. The influence of W/h on the φ factor is significant for creep-soft HAZ. The factor φ is higher for the larger HAZ width h (lower W/h ratio).

_{HAZ}and MF

_{WM}at the ratio W/h = 6.

_{HAZ}on φ are quite complex. For creep-hard HAZ (MF

_{HAZ}= 10), the values of φ are lower than one for all considered values of a/W. The value of φ becomes lower and asymptotically approaches a constant value as a/W increase. The value of MF

_{WM}has almost no effect on φ when a/W ≥ 0.7.

_{HAZ}= 1), the values of φ in the range 0.5 ≤ a/W ≤ 0.7 are higher than one if WM is creep-soft material (MF

_{WM}= 0.1). On the other side, for creep-hard WM (MF

_{WM}= 10) and range 0.5 ≤ a/W ≤ 0.7 the values of φ are lower than one. In both cases, for values of a/W > 0.7, the value of φ asymptotically approaches one. For creep match WM the value of φ is one for all considered values of a/W. This is expected because it is in fact a homogeneous material.

_{HAZ}= 0.1), the values of φ are significantly higher than one for all considered values of a/W. The value of φ becomes higher and asymptotically approaches a constant value as a/W increase. The value of MF

_{WM}has almost no effect on φ when a/W ≥ 0.7.

_{HAZ}and MF

_{WM}at the ratio W/h = 8. Thus, for a/W = 0.5 and MF

_{HAZ}= 10, the corresponding values of φ for W/h = 8 are higher than those for W/h = 6. Likewise, for a/W = 0.5 and MF

_{HAZ}= 0.1, the corresponding values of φ for W/h = 8 are lower than those for W/h = 6. In both cases, the value of φ asymptotically approaches a constant value as a/W increase. For a/W = 0.5 and MF

_{HAZ}= 1 and if WM is creep-soft material (MF

_{WM}= 0.1), the value of φ for W/h = 8 is higher than this for W/h = 6. For a/W = 0.5 and MF

_{HAZ}= 1 and if WM is creep-hard material (MF

_{WM}= 10), the value of φ for W/h = 8 is lower than this for W/h = 6. In the case where WM and HAZ are creep match materials, the value of φ is one for all considered a/W ratios.

_{HAZ}, MF

_{WM}and a/W for all W/h ratios, it can be generally concluded that there is a strong and complex influence of material and geometry constraints on the CCG rate. If the HAZ creep is a soft material, which is often the practice [18], the factor φ will have values higher than one. This means that the C* integral will be higher than the C* integral for homogenic material, so the CCG rate will also be higher. It is clear that a higher CCG rate means a shorter lifetime of the welded structure.

_{n}is quantity that depends on exponent n and the stress condition, ${\widehat{\sigma}}_{ij}$. and ${\widehat{\epsilon}}_{ij}$ are angular functions. Analyzing the diagrams in Figure 4, Figure 5 and Figure 6, it can be clearly concluded that the values of φ change with different combination of MF

_{HAZ}, MF

_{WM}, W/h and a/W. Different combinations of these parameters change the crack-tip constraint effect, and thus the magnitude of the crack-tip stress and strain rate. A higher magnitude of crack-tip stress and strain rate means a higher value of the C* integral, and thus a higher value of φ.

_{HAZ}, MF

_{WM}, a/W and W/h. This is the following expression:

## 4. Conclusions

## Author Contributions

## Funding

## Institutional Review Board Statement

## Informed Consent Statement

## Conflicts of Interest

## References

- Dake, Y.; Sridrah, I.; Zhongmin, Z.; Kumar, S.B. Fracture capacity of girth welded pipelines with 3D surface cracks subjected to biaxial loading conditions. Int. J. Press. Vessels Pip.
**2012**, 92, 115–126. [Google Scholar] [CrossRef] - Dake, Y.; Zhong, M.X.; Sridrah, I.; Kumar, S.B. Fracture analysis of girth welded pipelines with 3D embedded cracks subjected to biaxial loading conditions. Eng. Fract. Mech.
**2012**, 96, 570–587. [Google Scholar] - Xuan, F.-Z.; Tu, S.-T.; Wang, Z. A modification of ASTM E 1457 C* estimation equation for compact tension specimen with a mismatched cross-weld. Eng. Fract. Mech.
**2005**, 72, 2602–2614. [Google Scholar] [CrossRef] - Abe, F.; Tabuchi, M.; Tsukamoto, S.; Shirane, T. Microstructure evolution in HAZ and suppression of Type IV fracture in advanced ferritic power plant steels. Int. J. Press. Vessel. Pip.
**2010**, 87, 598–604. [Google Scholar] [CrossRef] - Dogan, B. Proceedings of CREEP8, Eighth International Conference on Creep and Fatigue at Elevated Temperatures (Joint with PVP07); University of Limerick: Limerick, Ireland, 2007; pp. 299–305. [Google Scholar]
- Tabuchi, M.; Hongo, H.; Watanabe, T., Jr.; Yokobori, A.T. Creep crack growth analysis of welded joints for high Cr heat resisting steel. ASTM Spec. Tech. Publ.
**2007**, 1480, 93–101. [Google Scholar] - Yatomi, M.; Fuji, A.; Tabuchi, M.; Hasegawa, Y.; Kobayashi KI, I.; Yokobori, T.; Yokobori, T. Creep crack growth of P92 welds. In Proceedings of the ASME 2008 Pressure Vessels and Piping Division Conference, Chicago, IL, USA, 27–31 July 2008; pp. 1207–1214. [Google Scholar]
- Hyde, T.; Saber, M.; Sun, W. Testing and modelling of creep crack growth in compact tension specimens from a P91 weld at 650 °C. Eng. Fract. Mech.
**2010**, 77, 2946–2957. [Google Scholar] [CrossRef] - Lee, K.-H.; Kim, Y.-J.; Yoon, K.-B.; Nikbin, K.; Dean, D. Quantification of stress redistribution due to mismatch in creep properties in welded branch pipes. Fatigue Fract. Eng. Mater. Struct.
**2010**, 33, 238–251. [Google Scholar] [CrossRef] - Tu, S.-T.; Segle, P.; Gong, J.-M. Creep damage and fracture of weldments at high temperature. Int. J. Press. Vessel. Pip.
**2003**, 81, 199–209. [Google Scholar] [CrossRef] - Tu, S.-T.; Yoon, K.-B. The influence of material mismatch on the evaluation of time-dependent fracture mechanics parameters. Eng. Fract. Mech.
**1999**, 64, 765–780. [Google Scholar] [CrossRef] - Xuan, F.-Z.; Wang, Z.-F.; Tu, S.-T. Creep finite element simulation of multilayered system with interfacial cracks. Mater. Des.
**2009**, 30, 563–569. [Google Scholar] [CrossRef] - Chen, G.; Wang, G.; Xuan, F.; Tu, S. Mismatch effect in creep properties on creep crack growth behavior in welded joints. Mater. Des.
**2014**, 63, 600–608. [Google Scholar] [CrossRef] - Chen, G.; Wang, G.; Zhang, J.; Xuan, F.; Tu, S. Effects of initial crack positions and load levels on creep failure behavior in P92 steel welded joint. Eng. Fail. Anal.
**2015**, 47, 56–66. [Google Scholar] [CrossRef] - Chen, G.; Wang, G.Z.; Xuan, F.Z.; Tu, S.T. Effects of HAZ widths on creep crack growth properties of welded joints. Weld. World
**2015**, 59, 851–860. [Google Scholar] [CrossRef] - Zhao, L.; Jing, H.; Xiu, J.; Han, Y.; Xu, L. Experimental investigation of specimen size effect on creep crack growth behavior in P92 steel welded joint. Mater. Des.
**2014**, 57, 736–743. [Google Scholar] [CrossRef] - Mehmanparast, A.; Maleki, S.; Yatomi, M.; Nikbin, K.M. Specimen Geometry and Size Effects on the Creep Crack Growth Behaviour of P91 Weldments. In Proceedings of the ASME 2013 Pressure Vessels and Piping, Division Conference, Paris, France, 14–18 July 2013. [Google Scholar]
- Li, Y.; Wang, G.Z.; Xuan, F.Z.; Tu, S.T. Geometry and Material Constraint Effects on Creep Crack Growth Behavior in Welded Joints. High Temp. Mater. Process.
**2016**, 36, 155–162. [Google Scholar] [CrossRef] - ASTM Standard, E1457-15. Standard Test Method for Measurement of Creep Crack Growth Times in Metals; ASTM International: West Conshohocken, PA, USA, 2015. [Google Scholar]
- ABAQUS /CAE 2016 User’s Manual. Inc. and Dassault Systems. Available online: http://130.149.89.49:2080/v2016/index.html (accessed on 15 June 2021).
- Katinić, M.; Konjatić, P.; Kozak, D.; Turk, D. Numerical analysis of the effect of residual stress on transient creep in SENB specimen. Int. J. Press. Vessels Pip.
**2020**, 188, 104222. [Google Scholar] [CrossRef] - Tada, H.; Paris, P.; Irwin, G. The Stress Analysis of Cracks Handbook; Paris Productions Inc.: St. Louis, MO, USA, 1985. [Google Scholar]
- Kumar, V.; German, D.; Shih, C.F. An Engineering Approach for Elastic-Plastic Fracture Analysis; EPRI Report NP-1931; EPRI: Washington, DC, USA, 1981. [Google Scholar]
- Goldman, N.L.; Hutchinson, J.W. Fully Plastic Crack Problems: The Center Cracked Strip Under Plane Strain. Int. J. Solids Struct.
**1975**, 11, 575–591. [Google Scholar] [CrossRef] - TuringBot Software, Sao Paulo, Brazil. 2021. Available online: https://turingbotsoftware.com/ (accessed on 12 August 2021).

**Figure 4.**Dependence φ factor on MF

_{HAZ}, MF

_{WM}and W/h for a/W = 0.5: (

**a**) MF

_{WM}= 10; (

**b**) MF

_{WM}= 1; (

**c**) MF

_{WM}= 0.1.

**Figure 5.**Dependence φ factor on MF

_{HAZ}, MF

_{WM}and a/W for W/h = 6: (

**a**) MF

_{HAZ}= 10; (

**b**) MF

_{HAZ}= 1; (

**c**) MF

_{HAZ}= 0.1.

**Figure 6.**Dependence φ factor on MF

_{HAZ}, MF

_{WM}and a/W for W/h = 8: (

**a**) MF

_{HAZ}= 10; (

**b**) MF

_{HAZ}= 1; (

**c**) MF

_{HAZ}= 0.1.

MF_{WM} | MF_{HAZ} |
---|---|

10 | 0.1 |

10 | 1 |

10 | 10 |

1 | 0.1 |

1 | 1 |

1 | 10 |

0.1 | 0.1 |

0.1 | 1 |

0.1 | 10 |

K_{I}(FE)/K_{I} | 1.005 | |

C*(FE)/C* | n = 5 | 0.978 |

n = 10 | 0.982 |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2021 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Katinić, M.; Turk, D.; Konjatić, P.; Kozak, D.
Estimation of *C** Integral for Mismatched Welded Compact Tension Specimen. *Materials* **2021**, *14*, 7491.
https://doi.org/10.3390/ma14247491

**AMA Style**

Katinić M, Turk D, Konjatić P, Kozak D.
Estimation of *C** Integral for Mismatched Welded Compact Tension Specimen. *Materials*. 2021; 14(24):7491.
https://doi.org/10.3390/ma14247491

**Chicago/Turabian Style**

Katinić, Marko, Dorian Turk, Pejo Konjatić, and Dražan Kozak.
2021. "Estimation of *C** Integral for Mismatched Welded Compact Tension Specimen" *Materials* 14, no. 24: 7491.
https://doi.org/10.3390/ma14247491